Research Article Phase Transformation of Iron Research Article Phase Transformation of Iron Oxide...
Embed Size (px)
Transcript of Research Article Phase Transformation of Iron Research Article Phase Transformation of Iron Oxide...
Research Article Phase Transformation of Iron Oxide Nanoparticles from Hematite to Maghemite in Presence of Polyethylene Glycol: Application as Corrosion Resistant Nanoparticle Paints
Pavani Katikaneani,1 Ajay Kumar Vaddepally,2 Narender Reddy Tippana,2
Ramu Banavath,2 and Srivani Kommu2
1Department of Chemistry, Rajiv Gandhi University of Knowledge Technologies-Basar, Telangana 504107, India 2Department of Metallurgical and Materials Engineering, Rajiv Gandhi University of Knowledge Technologies-Basar, Telangana 504107, India
Correspondence should be addressed to Pavani Katikaneani; email@example.com
Received 27 June 2016; Revised 23 July 2016; Accepted 25 July 2016
Academic Editor: Zhengjun Zhang
Copyright © 2016 Pavani Katikaneani et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
This work proposes a simple method for the efficient and rapid synthesis of hematite (𝛼-Fe 2 O 3 ) nanostructures based on simple
heating method under ambient conditions. Polyethylene glycol (PEG) is employed as a structure directing agent in driving the morphology and phase transformation. Typically, Fe
2 O 3 nanoparticles of size below 50 nmwere synthesized at temperature around
500∘C. The morphology and mechanism of formation of the nanocapsules and then aggregation of nanocapsules to form larger size nanoclusters were studied by scanning electron microscopy and energy dispersive X-ray spectroscopy. Interestingly, this work demonstrates the structural phase transformation of hematite (𝛼-Fe
2 O 3 ) to maghemite (𝛾-Fe
2 O 3 ) upon addition of different
amounts of PEG (say 0.066M, 0.133M, and 0.2M) and then heat treating at 500∘C.The prepared powders were used in nanoparticle paint preparation and applied as corrosion resistant coatings on iron samples. Polarization studies performed on the paint coatings made out of all the prepared samples showed size-dependent corrosion resistance. As the particle size decreases, the surface area increases and so the corrosion resistance also increases.
From the last few decades, transition metal oxide nanoparti- cles have attracted tremendous interest due to their promising applications as electrode materials for rechargeable solid- state batteries [1, 2], as efficient catalysts for fuel-cell reactions [3, 4], and as nanoscale magnetic models for understanding nanomagnetism [5, 6]. Amongst these, iron oxide nanopar- ticles have received much attention due to their massive applications in the fields of information storage disks, fer- rofluids, pigments, and medical applications like targeted drug delivery and cancer diagnoses [7–9]. Iron (III) oxide is an inorganic compound with the formula Fe
2 O 3 and it is
of one of the three main oxides of iron; the other two are rarely available iron (II) oxide (FeO) and naturally occurring iron (II, III) oxide (Fe
3 O 4 ). In steel industry, hematite is
the main source of the iron for the production of steel and it is paramagnetic, readily attacked by acids, and reddish brown in colour. As hematite is the most stable and n- type semiconductor under ambient conditions, it is widely used as catalysts, gas sensors, and pigments due to its high resistance to corrosion and low cost. It can also be used as a starting material for the synthesis of maghemite (𝛾-Fe
2 O 3 )
and magnetite (Fe 3 O 4 ), which have been intensively pursued
for technological applications in the last few decades . However, hematite is also interesting material as it has a band gap of 2.3 eV; the conduction band (CB) is composed of empty d-orbitals of Fe3+ and the valence band (VB) consists of fully occupied 3D crystal field orbitals of Fe3+ with some admixture from theO 2p nonbonding orbitals . Several methods to synthesize iron oxide nanoparticles such as mechanochemical [12, 13], wire electrical explosion ,
Hindawi Publishing Corporation Journal of Nanoscience Volume 2016, Article ID 1328463, 6 pages http://dx.doi.org/10.1155/2016/1328463
2 Journal of Nanoscience
Table 1: Experimental details.
Sample code Precursor 0.589M [Fe(NO 3 ) 3 ⋅9H 2 O] solution (mL) Amount of PEG in g Molar ratio(precursor : PEG)
Fe 2 O 3 -0 PEG 10 0 —
Fe 2 O 3 -4 PEG 10 4 (0.066M) 8.9 : 1
Fe 2 O 3 -8 PEG 10 8 (0.133M) 4.4 : 1
Fe 2 O 3 -12 PEG 10 12 (0.2M) 2.9 : 1
and electrochemical [15, 16] methods have been reported. On the other hand, the method employed in the present work is simple heating method in presence of PEG. Iron nitrate nonahydrate was used as a precursor to formulate Fe 2 O 3 nanostructures involving simple heating process with
varying amounts of PEG. The prepared samples were char- acterized by X-ray diffraction, field emission scanning elec- tron microscopy, and energy dispersive X-ray spectroscopy (EDX). Interestingly, powder XRD was found to show phase transformation from 𝛼-Fe
2 O 3 to 𝛾-Fe
2 O 3 with the increase in
PEG concentration.This type of transformation is commonly observed with the effect of temperature [17, 18].The prepared nanoparticles were used in paint preparation and were found to show excellent corrosion resistance as coatings.
2. Experimental Method
2.1. Synthesis. Iron oxide nanoparticles (Fe 2 O 3 ) are prepared
by simple heating method. This process involves prepara- tion of 0.589M solution of ferric nitrate nonahydrate salt precursor by dissolving 10 g of Fe(NO
3 ) 3 ⋅9H 2 O in 42mL
water to precipitate the oxohydrate at higher temperatures (∼70∘C). To each 10mL of prepared salt precursor solution, various amount of PEG (0M, 0.066M, 0.133M, 0.2M) (as shown in Table 1) is added and stirred for one hour at higher temperatures (∼100∘C) till the homogeneous viscous solution is formed.These viscous materials were heat treated at 500∘C for 1 hour to obtain different iron oxide nanopowders.
2.2. Characterization. The crystal structure of the synthe- sized particles was determined by powder X-ray diffrac- tometer (D8 Discover, Bruker AXS Co., Ltd., Germany) with Cu-K𝛼 radiation, 𝜆 = 1.54056 Å. The particle size and morphology were derived from field emission gun scanning electron microscope (Carl Zeiss Co. Ltd., Germany) and the elemental composition was obtained from energy dispersive X-ray spectroscopy attached to FESEM (EDX INCA, Oxford Instruments).
2.3. Corrosion Study
2.3.1. Paint Preparation. Paint preparation involves (i) pig- ment preparation, (ii) binder preparation, and (iii) pigment binder grinding. Pigment preparation is carried out by taking prepared iron oxide nanoparticles of 1 g each (Fe
2 O 3 -0 PEG,
Fe 2 O 3 -4 PEG, Fe
2 O 3 -8 PEG, and Fe
2 O 3 -12 PEG) onto a glass
slab and made into paste using linseed oil. The iron oxide
particles were taken onto a glass slab and then a crater ismade in themiddle of the powder, into the crater 1mL of linseed oil is poured, and the mixture was mixed thoroughly with pallet knife. Along with this, binder is prepared by the addition of 2% of bee wax in the linseed oil. For this purpose, 0.4 g of bee wax is added to 19.6mL of linseed oil and the mixture was heated at 60∘C along with magnetic stirring, until all the wax gets dissolved in linseed oil and the colour of mixture turns out to be yellowish.This is cooled to room temperature and can be used as binder. Once the binder cools to room temperature, the pigment is taken onto glass slab; few drops of binder are added and ground well using a miller till the pigment gets mixed up with binder and feels like paint. The prepared paint is stored in plastic containers and was coated on thin sheets of iron on one side and tested for polarization curves.
2.3.2. Potentiodynamic Polarization Curve. A characteristic three-electrode electrochemical corrosion cell was used in all the experiments. As a reference, a saturated calomel electrode (SCE) was used. All measured potentials were referred to this electrode. A platinum foil was used as the counter electrode. Then (i) parent iron sample (blank uncoated sample) and iron samples coated with paints prepared out of (ii) Fe
2 O 3 -0
PEG, (iii) Fe 2 O 3 -4 PEG, (iv) Fe
2 O 3 -8 PEG, (v) Fe
2 O 3 -12 PEG,
and (vi) microsized Fe 2 O 3 powder were used as working
electrodes. A potentiostat (IEC 61326, Ivium Technologies, Netherlands), controlled by a personal computer, equipped with aGPIB card and the commercial software, was employed to attain the potentiodynamic polarization curves. Before every experiment, the open circuit potential (OCP) was recorded for at least 30 minutes. Polarization curves were obtained potentiodinamically; the linear potential sweep was performed at a ±248mV potential window around the measured OCP, from the cathodic to the anodic side, at scan rates of 0.1 and 1mV s−1.
3. Results and Discussion
3.1. Powder XRD. The powder X-ray diffraction (XRD) was performed to identify the phase composition of nanoparti- cles. Iron oxides havemany phases such asmagnetite (Fe
3 O 4 )
and maghemite (𝛾-Fe 2 O 3 ) with cubic crystal structure and
hematite (𝛼-Fe 2 O 3 ) with rhombohedral crystal structure.
The magnetite and maghemite have black and light brown colours, respectively , due to the similar crystal structure and close lattice parameters (𝑎 = 8.396 Å for magnetite and
Journal of Nanoscience 3
20 30 40